HAL Id: hal-01680756
Submitted on 7 Nov 2019
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.
Compaction behavior of binary mixtures
Abderrahim Michrafy, Harona Diarra, John A. Dodds
To cite this version:
Abderrahim Michrafy, Harona Diarra, John A. Dodds. Compaction behavior of binary mixtures.
Pow-der Technology, Elsevier, 2009, 190 (1-2), pp.146-151. �10.1016/j.powtec.2008.04.066�. �hal-01680756�
Compaction behavior of binary mixtures
, H. Diarra, J.A. Dodds
RAPSODEE (UMR CNRS 2392), Ecole des Mines d'Albi-Carmaux, Campus Jarlard, 81000 Albi, France
A B S T R A C T Keywords: Die-compaction Binary mixtures Densiﬁcation Radial stress Friction Capping
The compaction behavior of binary mixtures of lactose and a functional excipient containing 98% of microcrystalline cellulose and 2% of silica was investigated by experiment. The densiﬁcation process and the role of each component in the compaction behavior were examined by analyzing the effect of the composition on the stress transmission to the powder bed in axial (stress transmission) and in radial (stress transfer) directions. Unlike the behavior of a single component where the applied pressure is predominantly transmitted in the axial direction to the powder bed for densiﬁcation, the increase of the composition of lactose up to 50% in mixtures increases the stress transfer that becomes greater than the stress transmission. However, for the compaction behavior of mixtures with 50% of lactose, two opposite behaviors were found, below and above a pressure around 70 MPa. Die-wall friction showed also a change at this pressure due to a smoothed contact surface with wall. By increasing the composition of lactose (N50%), the behavior of mixtures becomes dominated by the behavior of lactose where the transmission is better than the transfer. This study demonstrates that the analysis of the compaction behavior of mixtures by recording stress transmission, stress transfer and wall friction give pertinent information about the role of each component in the densiﬁcation and could be, to a certain extent, help to the selection of excipient for powder formulation.
The die-compaction is a size enlargement process for particulate solids to produce tablets with sufﬁcient strength for storage and handling. This process which is economic and ensures a good stability for tablets, is widely used in pharmaceutical industry. Pharmaceutical tablets are often manufactured from several powders and it is of interest to analyze the tablet properties according to the formulation. In the ﬁeld of the compaction of binary mixtures, several recently studies were reported in the literature and concerned properties of the tablets such as the evolution of compacted binary mixture porosity, the solubility, the tensile strength[3–5], or the com-pressibility of the mixtures. However, the role of each component in the densiﬁcation process and in the capping problem of tablets was not considered.
The present paper reports on the densiﬁcation behavior of binary mixed powders of lactose and a functional excipient containing 98% of microcrystalline cellulose and 2% of silica during die-compaction according to the components. The goal is to propose an analysis based on wall friction and stress transmission in axial and radial directions to investigate the behavior of each component in the mixture during the compaction.
2. Materials and Methods 2.1. Instrumented press 2.1.1. Instrumentation
The apparatus used for the compaction was a reciprocating tablet press (Frogerais OA). The pressure is applied with the upper punch and the ejection with the lower one. The upper and the lower punches are instrumented by strain gauges measuring pressures and by LVDT sensor for the relative displacement between punches. A ﬁxed cylindrical die of 11.28 mm of diameter and 10 mm of height was modiﬁed as shown inFig. 1and was equipped with a strain gauge (Wheatstone bridge circuit) mounted on the die wall. The gauge was placed at 1.5 mm from the surface of the lower punch so that at end of the compaction, the gauge is approximately positioned at the middle of tablets with height in the range 3–4 mm.
The geometry of the die allows the increasing of the sensitivity of the system. Also, this system offered the advantage of not altering the sensor as in the instrumentation with load cell in contact with the powders (particularly the ﬁne and cohesive powders).
2.1.2. Calibration of radial gauge
A rubbery material was chosen for the calibration because it behaves as very nearly hydrostatically under pressure. Thin discs of 1 mm thickness and 11.28 mm diameter were cut from rubber material using a concave punch (for its cutting capability). As the height of the chamber of the die is as 10 mm, ﬁve curves (pressure in
⁎ Corresponding author. Tel.: +33 56349 3162; fax: +33 56349 3025. E-mail address:firstname.lastname@example.org(A. Michrafy).
MPa vs signal in mV) were generated according to the height of stacked discs. Each curve was generated from 20 data measurements. The generated curves corresponding to heights 2, 4, 6, 8 and 10 mm were linear and their slopes were determined for the conversion of the signal of radial gauge in mV to a pressure in MPa. It should be noted that the maximum applied pressure was limited to 120 MPa to avoid the creep problem of thin discs. For a given height of tablet, the radial pressure was obtained by interpolating data from the calibra-tion curves.
2.2. Binary mixtures preparation
Two powders used as excipients in the pharmaceutical formula-tions were selected for the binary mixtures: a lactose powder (lactose Granulac® 140 from Meggle GMBH) and a functional excipient noted ‘smcc’ containing microcrystalline cellulose 98% and silica 2% (Pro-solv® 90 from J. Rettenmaier & Shöne). The lactose is known for its fragmentary behavior with compression and its bad ﬂow, whereas the powder ‘smcc’ behaves like microcrystalline cellulose (plastic beha-vior) and has a good ﬂow. A Scanning Electron Microscopy image of these powders is presented inFig. 2and shows the rough surface of smcc. This suggests favorable contact conditions of particles. The basic characteristics (average size of particles, true density and bulk density) of the studied powders are summarized in theTable 1.
Various mass fractions (15, 25, 35, 50, 60 and 75% of lactose in mass) in lots of 100 g were blended and were thoroughly mixed in a Turbula mixer (Turbula®, System Schatz, Basel Switzeland) during 5 min with 32 rpm.
2.3. Compaction of mixtures
Cylindrical ﬂat tablets have been made from these powders by the following procedure. 100 g lots of mixtures were put in the hopper of the reciprocating press just after the mixing operation. During the compaction process, a mass of 0.45 ± 0.02 g of powder was poured in the die and compacted at different pressures using the instrumented reciprocating tablet press making it possible to record the pressure and displacement on the top and the bottom punches as well as the radial stress on the die. The compaction was made at the speed around 31 mm/s at the ambient temperature of 25 °C ± 1 °C and 64% of relative humidity. Once the tablet was ejec-ted, its mass was measured with an electronic balance (CP 224S, Sartorius Germany). For each pressure, six compacts were made using the above procedure. To avoid die ﬁlling problems at the start of compaction run, only the last three compacts were considered in measurements. Each measurement presented here was the mean of the characteristics of three tablets. The maximum errors on pressures depended on the proportion of lactose in mixtures. For lactose composition lower 50%, maximum of errors were as 2.8% for applied pressure, 0.4% for transmitted pressure and 2.9% for radial pressure. For composition greater than 50% of lactose, errors were as
3.4% for applied pressure, 0.5% for transmitted pressure and 4.1% for radial pressure.
2.4. Stress transmission and stress transfer ratios
During die-compaction of a powder mass, the axial stress applied by the upper punch is transmitted to the powder causing its densiﬁcation in axial direction whereas a stress is developed in die cavity by expansion in normal direction to die wall and measures the densiﬁcation in radial direction. The stress transmitted to the lower punch is sensed and is less than the applied pressure because the existence of an opposite stress on the powder bed due to wall friction. The capacity of a powder mass to convert the applied pressure to the axial and radial densiﬁcation is a characteristic of the behavior of the
Fig. 1. (a) Schematic drawing of instrumented die, dimension in mm, (b) picture of modiﬁed die.
Fig. 2. Scanning Electron Microscopy images of powders (a) lactose Granulac 140 (Meggle Gmbh) and (b) Prosolv® 90 (J. Rettenmaier & Shöne).
powder. In this way Shaxby and Evans introduced the ratio of transmitted to applied pressure as a logarithmic relationship of thickness, diameter of the tablet and a material constant. In the work of Unckeland Toor et al.the ratio of radial to axial pressure was included in the above relationship.
In this study, the stress transmission and transfer deﬁned as: Transmission ¼ σl=σu ð1Þ and the stress transfer expressed as
Transfer ¼ σr=σu ð2Þ
were used as indices quantifying capabilities of mixtures to favor axial transmission or radial transfer during the compaction cycle. They were also used as tools to analyze mechanisms of the densiﬁcation and the anisotropy of the stress transmission generated in the powder bed. 2.5. Residual radial stress and capping analysis
The radial to axial pressure of the compaction cycle has been studied by different authors[11–13]. They show the interest of the analysis of the proﬁle of radial to axial pressure in the characteriza-tion of the compaccharacteriza-tion properties of powders and the analysis of lamination and capping problems. In the context of this study, the proﬁle of the radial to axial pressure in cycle compression was analyzed according to the composition of binary tablets. From experimental data, it was found that the residual radial stress could not explain capping observed for compositions of lactose higher than 50%. It was however suggested examining the decrease of radial stress when the axial pressure reached zero (σr,1) and just
before starting the ejection (σr,2). During this period, the tablet is
yielding continuously in shear and its magnitude (relatively to the pressure) was expressed as:
RRS ¼ σ! r;1−σr;2"=σu: ð3Þ
The ratio RRS as “Restituted Radial Stress” has been used to analyze the capping according to composition.
2.6. Die-wall friction
The friction between the mixtures and die wall was examined to explain the behavior of certain compositions. Coulomb friction was assumed at die wall, i.e. the friction traction was assumed proportional to the traction at normal direction to the die wall. The friction coef-ﬁcient μ (σr) was evaluated from radial pressure σrand pressures on the upper σu and the lower σlpunches at end of the compaction
(maximum pressure) as:
μ σð Þ≈ σr ð u−σlÞ=σr: ð4Þ
Basic characteristics of lactose and smcc
Powders d50(μm) Apparent density (g/cm3) True density (g/cm3)
smcc 90 0.32 1.598± 0.003
lactose 70 0.66 1.561± 0.0022
Restituted residual radial stress (RRS) versus composition of lactose (binary mixtures smcc + lactose)
Lactose% σu[MPa] σr,1[MPa] σr,1[MPa] RRS (%)
15 115 17.5 14.5 2.6 25 127 18 15.5 1.97 35 112 17.6 14.7 2.59 50 116 22 15.5 5.60 65 94 16.1 11.7 4.68 75 111 19 13 5.40
Fig. 3. a) Radial stress vs axial pressure. Compaction of 25% lactose+ 75% smcc at pressure 103 MPa. b) Radial stress vs axial pressure. Compaction of 50% lactose+ 50% smcc at pressure 109 MPa. c) Radial stress vs axial pressure. Compaction of 75% lactose+ 25% smcc at P= 111 MPa.
Fig. 4. a) Transfer and transmission ratios versus pressure (0% lactose). b) Transfer and transmission vs pressure (15% lactose). c) Transfer and transmission vs pressure (25% lactose). d) Transfer and transmission vs pressure (35% lactose). e) Transfer and transmission vs pressure (50% lactose). f) Transfer and transmission vs pressure (60% lactose). g) Transfer and transmission vs pressure (75% lactose).
The analysis of die-wall friction from Eq. (3) was complementary to information obtained from the above indices on the behavior of mixtures.
3. Results and discussions 3.1. Radial vs axial pressure
InFig. 3(a–c) are plotted the evolution of the radial stress versus the applied pressure for the composition 25, 50 and 75% of lactose during the loading and the unloading steps. The maximum pressure was respectively 103, 109 and 111 MPa. In the loading phase, the radial and axial pressure proﬁles were linear. The slope of curve was 0.6 (resp. 0.68) for the composition 25% of lactose (resp. 50 and 75% of lactose). In the decompression step and after the release of the pressure the tablet remained in the die under an appreciable residual radial stress ((σr,1=15 MPa for mixture with 25% of lactose, (σr,1=
20 MPa for mixtures with 50 and 75% of lactose). According to these values, the residual radial stress could not explain the capping observed in tablets with lactose compositions higher than 50%. As the tablet was yielding continuously in shear during the short time between the release of the pressure and the ejection steps, the Restituted Radial Stress (RRS) from the Eq. (3) was used as an alternative to explain the capping observed for composition with lactose higher than 50%. In Table 2 are reported, values of RRS according to the composition. As it can be seen two groups may be distinguished: a group with RRS between 2 and 2.6% for mixtures of lactose lower 50% and a group with RRS between 5.4 and 5.7% for compositions with more than 50% of lactose: “The greater the RRS and the weaker the tablet is weak, more is capping potentially possible”. The RRS could be used as criteria of capping if the fracture limit of tablet under shear could be characterized.
3.2. Densiﬁcation behavior of binary mixtures
The behavior of binary mixtures in compaction was analyzed using the stress transmission (Eq. (1)) and stress transfer (Eq. (2)). During die-compaction, the evolution of these ratios was simultaneously represented inFig. 4(a–g) according to the axial pressure for com-position 0, 15, 25, 35, 50, 65 and 75% of lactose. In the case of the single powder compaction of smcc (Fig. 4a), the transmission was typically 76% whereas the transfer ratio was lower than the transmission and reached 60%.
The addition lactose powder in the mixture in proportions lower than 50%, (Fig. 4(b–d)) show the opposite situation with the transfer higher than the transmission, i.e. the densiﬁcation seems more oriented out of the axial axis. The case of mixture 50–50% inFig. 4e shows two steps according to the pressure level: for pressure b70 MPa, the stress transfer decreased and was higher than the stress transmission which increased. However, for pressure N70 MPa, the situation was inversed. This change was also found in the evolution of wall friction (Fig. 5b) where the friction coefﬁcient decreased rapidly at 70 MPa meaning the change of properties of the contact. Probably for this composition and around 70 MPa, the lactose powder played a lubricant role (by coating contact surface under pressure).
For lactose contents greater than 50% (Fig. 4f–g), the behavior was reversed and stress transmission was higher than stress transfer resulting from the dominant composition of lactose powder that have a good stress transmission in axial direction.
3.3. Die-wall friction
The wall friction coefﬁcient was evaluated using Eq. (4), for the studied mixtures and its evolution with radial pressure is plotted in
Fig. 5a for mixtures 0, 15, 25 and 35% of lactose. For smcc alone, the wall friction coefﬁcient was as 0.4 and decreased slightly with radial pressure.
This value is in agreement with data of other microcrystalline cellulose
. It is also shown inFig. 5a that, the addition of lactose powder to smcc in proportions lower than 50% increases the friction coefﬁcient due to the high radial pressure generated for such mixtures (stress transfer ≈70%). On the other hand, for mixtures with lactose compositions greater than 50% (Fig. 5c), the friction coefﬁcient was lower than 0.2. The
Fig. 5. a) Wall friction vs radial pressure (mixtures with 0, 15, 25 and 35% of lactose). b) Wall friction vs radial pressure (50% of lactose). c) Wall friction vs radial pressure (mixtures with 60% and 75% of lactose).
case of equal compositions (Fig. 5b) showed a transition in the compaction behavior around 70 MPa of applied pressure (50 MPa of radial pressure). Below this pressure, the friction coefﬁcient increased up to 0.61 and decreased rapidly down to 0.2 after. This means a change in the contact properties at the interface between die wall and tablet. 4. Conclusion
The densiﬁcation behavior of binary mixed powders (lactose and a functional excipient containing 98% of microcrystalline cellulose and 2% of silica) during die-compaction is analyzed from measure-ments obtained with an instrumented press equipped with radial gauge. Indices such as stress transfer, stress transmission and wall friction coefﬁcient were analyzed according to the pressure and composition of lactose powder in mixtures. It is shown that there is a change of the densiﬁcation behavior with the lactose content. High composition (N50% in mass) of lactose in mixtures favors the transmission load in the axial direction, but the resulting tablets have laminations that can be explained from the magnitude of Restituted Radial Stress (RRS) under which tablet is continuously yielding in shear. In the other mixtures with high composition of cellulose favor the compaction in radial direction and present low values of RRS limiting the shearing solicitations after the release of pressure and before ejection. The compaction of a 50:50 mixture shows the role of the pressure in the change of the densiﬁcation behavior particularly by modifying interfacial properties between tablet and die wall. The analysis proposed here on the densiﬁcation of binary mixtures could be also employed for the selection of excipients for formulation step.
List of symbols
σu Pressure on upper punch
σl Pressure on lower punch
σr Radial pressure (on die)
σr,1 Residual radial pressure just after release of
σr,2 Residual radial pressure just before ejection
RRS=(σr,1−σr,2)/σu Restituted Radial Stress
μ(σr)≈(σu−σl)/σr Die-wall friction (Coulomb friction)
σl/σu Stress transmission ratio
σr/σu Stress transfer ratio
 J.-C. Masteau, G. Thomas, Evolution and modelling of compacted binary mixture porosity. Application to pharmaceutical tablets, J. Chim. Phys. 96 (7) (1999) 1245–1268.
 H. Leuenberger, Compression of binary powder mixtures and solubility para-meters of solids, Int. J. Pharm. 27 (1985) 127–138.
 N. Ramirez, L.M. Melgoza, M. Kuentz, H. Sandoval, I. Caraballo, Comparison of different mathematical models for tensile strength-relative density proﬁles of binary tablets, Eur. J. Pharm. Sci. 22 (2004) 19–23.
 C.-Y. Wu, S.M. Best, A.C. Bentham, B.C. Hancock, W. Bonﬁeld, A simple predictive model for the tensile strength of binary tablets, Eur. J. Pharm. Sci. 25 (2–3) (2005) 331–336.
 A. Michrafy, M. Michrafy, M.S. Kadiri, J.A. Dodds, Predictions of tensile strength of binary tablets using linear and power law mixing rules, Int. J. Pharm. 333 (2007) 118–126.
 V. Busignies, B. Leclerc, P. Porion, P. Evesque, G. Couarraze, P. Tchoreloff, Compaction behaviour and new predictive approach to the compressibility of binary mixtures of pharmaceutical excipients, Eur. J. Pharm. Biopharm. 64 (2006) 66–74.
 B.E. Sherwood, J.W. Becker, A new class of high functionality excipients: siliciﬁed microcrystalline cellulose, Pharm. Technol. 10 (October 1998) 78–99.
 J.H. Shaxby, J.C. Evans, Trans. Faraday Soc. 19 (1923) 60.  H. Unckel, Arch. Eisenhutt Wes. 18 (1945) 161.  H.L. Toor, S.D. Eagleton, Ind. Eng. Chem. 48 (1956) 825.
 W.M. Long, Radial pressures in powder compaction, Powder Metall. 6 (1960) 73.  S. Leight, J.E. Carless, B.W. Burt, Compression characteristics of some
pharmaceu-tical materials, J. Pharm. Sci. 56 (1967) 888–892.
 K. Sugimori, S. Mori, Characterization of die wall pressure to predict capping of ﬂat or convex-faced drug tablets of various sizes, Powder Technol. 58 (1989) 259–264.  A. Michrafy, M.S. Kadiri, J.A. Dodds, Wall friction and its effects on the density distribution in the compaction of pharmaceutical excipients, Trans. IchemE 81 (2003) 946–951 (Part A).